The few layer transition metal dichalcogenides are two dimensional materials that have an intrinsic gap of the order of ≈2 eV. The reduced screening in two dimensions implies a rich excitonic physics and, as a consequence, many potential applications in the field of opto-electronics. Here we report that a layer perpendicular electric field, by which the gap size in these materials can be efficiently controlled, generates an anomalous inter-layer exciton whose binding energy is independent of the gap size. We show this originates from the rich gap control and screening physics of TMDCs in a bilayer geometry: gating the bilayer acts on one hand to increase intra-layer screening by reducing the gap and, on the other hand, to decrease the inter-layer screening by field induced charge depletion. This constancy of binding energy is both a striking exception to the universal reduction in binding energy with gap size that all materials are believed to follow, as well as evidence of a degree of control over inter-layer excitons not found in their well studied intra-layer counterparts.
The experimental fabrication of graphene in 2004 marked the onset of a new science of low dimensional materials. Of the many materials that have followed graphene, one of the most remarkable has been the few layer transition metal dichalcogenides1,2,3 (TMDCs). Similar to graphene in some ways, for instance both have a valley degree of freedom4, these materials differ in a number of key respects. While graphene is a semi-metal the TMDCs have an intrinsic band gap, an inheritance from the bulk crystal which is a semi-conductor. Furthermore, a high degree of control over this gap exists in bilayer TMDCs5, with theory6,7 reporting that layer perpendicular electric fields of only 2–3 V/nm can close a gap of ≈2 eV. As a band gap plays a crucial role in the on-off ratio of field-effect transistors, the presence of an intrinsic and controllable band gap is a profound technological advantage8,9. Most importantly, the TMDCs host a rich physics of excitons (a bound state formed of a valence band hole and a conduction band electron) with exceptionally large binding energy5,10,11,12,13,14,15,16. This opens up a vast arena of potential opto-electronic applications for these materials17. In this paper, through the example of MoS2, we will investigate the theory of the interplay between these two key aspects of TMDCs: the electric field control of the band gap and the excitonic physics.
Theoretical understanding of the TMDCs is non-trivial. Firstly, there are many indications that electron correlation plays a decisive role in the properties of these materials6,18, a point of view we will richly confirm in this paper. Secondly, excitonic physics by its very nature demands a many-body treatment. A standard density functional theory approach will not suffice for the investigation of these materials and recourse must be made to the full machinery of many-body physics: the GW method must be deployed for the ground state followed by the solution of the Bethe-Salpeter equation19 (BSE), or a time dependent density functional theory20, to access the excitonic physics. These many-body techniques are computationally very demanding and thus only a few such calculations6,21,22 exist, all of which are for the case of zero electric field.
A recent experimental investigation reports an intriguing excitonic physics of MoS2 in the presence on a layer perpendicular electric field, with intra- and inter-layer excitons appearing to behave quite differently5. It is the purpose of the present paper to apply the full “tool kit” of many-body ab-initio science (GW in conjunction with the BSE) to this system, and to fully reveal the remarkable nature of this excitonic physics of MoS2 in an electric field.
Results and Discussion
Band gap engineering
The behaviour of bilayer MoS2 in a layer perpendicular electric field has been well established by DFT studies: the band gap can be continuously reduced with increasing field strength5,23,24,25. This tuning of the band gap is so dramatic that both (i) a transition from indirect to direct band gap and (ii) full metalization can be observed (at 1–2 V/nm and 2–3 V/nm respectively, depending on the stacking type of the bilayer). As the ground state spectrum is known to be strongly - and non-uniformly - renormalized by many-body effects, we will first revisit the band gap behaviour using the GW method. In Fig. 1 we present both DFT (we deploy the PBE functional) and GW calculations of the band gap as a function of field; we show results only for the AA′ stacking, known to be the lowest energy stacking configuration26 of the MoS2 bilayer. Clearly, many-body effects play a crucial role in the behaviour of the band gap: while the gap reduces at 604 meV per unit field with the DFT calculation (in good agreement with earlier work23,25, this value is almost half −384 meV - if many-body effects are included via the GW method. These GW results are much closer to the experimental value5 of 260 meV per unit field. We also note that the band gap error from the DFT calculation appears to be increasing with field: an error of 30% at zero field becomes an error of almost 70% at 2 V/nm. This strongly suggests that many-body effects are both crucial to the treatment of bilayer MoS2 in an electric field, and indeed become more important with increasing field. As the difference between the two methods lies in the much better treatment of screening in the GW method, and as excitonic physics depends crucially on the screening of the excitons, we conclude that a GW treatment of the ground state is essential.
Field induced excitonic physics
The imaginary part of the dielectric function ε2, calculated by solving the BSE, is exhibited in Fig. 2 for a range of electric fields. Below the fundamental gap and in absence of the electric field ε2 is dominated by two main excitonic peaks, marked as A and B at energies 1.99 eV and 2.19 eV respectively (these peak positions are in excellent agreement with previous theoretical works18,21). When the field is applied two things occur: (a) the A and B peaks split, but otherwise remain largely unchanged in energy as the field changes and (b) above a critical field of 0.3 V/nm a new spin - orbit split excitonic peak (II-1 and II-2) emerges whose resonance energy changes strongly as a function of field. The second of these features is the novel interlayer excitonic peak described in the experimental work of Chu et al. (the spin - orbit splitting is likely too small to have been observed, see the broad peaks in Fig. 4c and error bars in Fig. 4e of ref. 5). While the experiment clearly observed a dramatically different behaviour of peak positions A and II, measurement accuracy precluded a statement being made about the binding energies (difference between the gap and the position of the excitonic peak) of these excitons. Theoretically we have no such restriction, and can now proceed to a careful analysis of this novel excitonic behaviour.
We first confirm the intra- and inter-layer character of the exciton types A and II. This may be easily checked as it is well established that all bands near the gap approach pure layer character as the field increases. Thus by restricting the sub-space in which the Bethe-Salpeter equation is solved to conduction and valence manifolds from the same, or different, layers we may immediately deduce which excitons result from intra- or inter-layer transitions. We are thus, in this way, able to confirm that exciton peak A (and B) are purely intra-layer excitons, while exciton peak II is an inter-layer exciton.
Having established this, in Fig. 3(a) we first present the peak position as a function of applied field, finding agreement with experiment in the fact that the A-1 and A-2 peaks remain almost unchanged with field while, on the other hand, the position of the II-1 and II-2 peaks changes strongly. The absolute positions of all resonances are blue shifted with respect to experiments5,10 by ~0.14 eV, a fact that has already been noticed at zero field21. This deviation from experiment is almost independent of the applied field, and we therefore find a rate of change of peak II with applied field to be very close to the experimental value of 275 meV per unit field (the best find line to the theoretical data yields 384 meV per unit field). We now turn to the binding energy of excitons A and II, presented in Fig. 3(b). Remarkably, the evolution in the position of peak II with field is almost perfectly compensated by a corresponding change in the band gap. On the other hand the constant peak position of exciton A-2, due to the changing band gap, corresponds to a continuously reducing binding energy with field (exciton A is not bound for field values ≥0.6 V/nm). We therefore conclude that the trends in binding energy - the physically relevant property of the exciton - are the opposite of the peak position trends: the binding energy of exciton II is weakly dependent on the field, while that of A is strongly dependent on the field.
An exciton binding energy that is almost independent of the gap is a strikingly anomalous behaviour, a point that may be vividly brought out by comparison to the gap dependence of binding energies found generally in two dimensional materials. In Fig. 4(a) we present the binding energy as a function of gap size for a wide range of two dimensional materials. In the absence of the anomalous exciton II, all binding energies fall close to a best fit line, a universal behaviour first noticed by Choi et al.27. In Fig. 4(a) we include several additional materials to those considered in ref. 27 which both changes the slope of the universal line and worsens the fit, however to a good approximation the linear law still holds. What lies behind this universal relation discovered by Choi et al. To answer this in panel (b) of Fig. 4 we present macroscopic ε−1 (ω → 0, q = 0) - a direct measure of the screening - plotted against the gap size for a diverse set of materials (including both two and three dimensional cases). An almost perfect universal linear behaviour can be observed, and thus the linear law for the exciton binding energy27 represents a manifestation of a deeper linear screening law. The constancy of the binding energy of exciton II as a function of the band gap in bilayer MoS2, in conjunction with the “regular” behaviour of exciton A, is therefore indicative of an unusual screening physics.
To further elucidate this physics we note that in an increasing electric field the charge accumulates in-plane while being depleted from the interlayer region23. As a consequence of this field induced change in charge density intra-layer screening will become stronger with increasing field (more charge to screen with) while, at the same time, having a tenancy to reduce inter-layer screening (less charge to screen with). This explains the binding energy trend of both excitons: the in-plane exciton (A) is “screened away” due to this increased intra-layer screening while, in contradistinction, once the interlayer screening is sufficiently weak the binding energy of exciton II is insensitive to further reduction in screening. This critical value occurs at a field strength of ≤0.3 V/nm and below this value distinct II and A excitons cannot be determined. By performing a BSE calculation in the subspace of only inter-layer bands we confirm that the exciton II is created at a field of 0.18 V/nm.
It is important to mention that the new inter-layer exciton II is bright but, as is already clear from Fig. 2, comes with a very low intensity. To probe this further we plot in Fig. 5 the oscillator strength (OS)19 for peak II as a function of field. Evidently, the exciton II OS is not only very low, for instance at 0.1 V/nm the OS for peak A is about 20 times greater, but furthermore continuously reduces with increasing field strength; at 1.5 V/nm this ratio of oscillator strengths is 140. These results are in perfect consonance with the experimental finding of a very low photoluminescence yield for the inter-layer exciton as compared to the intra-layer exciton.
Summary and Discussion
Gating the bilayer creates a new inter-layer charge transfer exciton, recently reported in experiments5. We find excellent agreement with experimental measurements of the exciton peak positions, and in addition our theoretical analysis affords considerable additional insight into the nature of the excitonic physics. In particular, we find that the interlayer exciton (II) has a binding energy that is, quite remarkably, independent of the gap size. We trace this anomalous behaviour to the fundamental screening physics of the bilayer: an electric field acts to increase intra-layer screening but decrease inter-layer screening. This new excitonic physics is therefore tied to the basic physics of a gated bilayer geometry, and goes beyond the example we have presented. We conclude that the electric field induced excitonic physics of the TMDC bilayers will exhibit two distinct types of excitonic behaviour: (i) in-plane excitons will become, following the universal trend, less strongly bound as the field closes the gap but, (ii), inter-layer excitons will not follow this universal trend, and the binding energy will be unchanged once the inter-layer screening falls below some critical value. The electric field induced excitonic physics of bilayer TMDCs therefore offers an unexpectedly rich degree of control over the exciton binding energy, a feature that may be of considerable importance in opto-electronic applications.
The calculations are performed using a super-cell geometry with a large vacuum21 of 30 Å (56.7 a.u.) and an in-plane lattice parameter fixed to the bulk experimental value of 3.160 Å28. The details of the AA’ stacked configuration that we calculate may be found in ref. 26. We fix the interlayer separation to the same value at all fields; the gap reduction of the GW calculations (but not the DFT calculations) is then found to agree closely with experiment. We note that relaxing this constraint has, in one work25, been reported to dramatically impact the gap reduction with field, however in such a way that brings the results into sharp disagreement with experiment5.
Electronic structure calculations
The ground-state density functional theory (DFT) calculations are performed using the Perdew-Burke-Ernzerhof (PBE)29 exchange-correlation functional using the PAW method as implemented in the VASP30 code. We have employed the non-self-consistent GW method31 to determine the many-body gaps, with excitonic properties calculated by solving the Bethe Salpeter equation (BSE)19 in the q → 0 limit. Optical spectra was calculated using an energy cutoff of 400 eV, a Gaussian smearing of 0.02 eV, 200 unoccupied bands, and a force tolerance of 0.01 eV/Å. We have included 50 G-vectors to account for local field effects. Spin-orbit interaction is included in all calculations. The ELK code32 has been deployed to verify the veracity of the BSE results.
In order to obtain reliable binding energies it is of vital importance to fully converge the optical spectra. As in a previous work21, we find that excitonic binding energies are very sensitive to the number of k-points. As is clear from Fig. 6 a minimum grid of 18 × 18 × 1 is required to obtain reliable binding energies (to an accuracy of 0.01 eV), which are then fully converged at a grid size of 24 × 24 × 1. Hence all the results presented in previous sections are calculated using a k-point grid of 24 × 24 × 1.
The electric field is included as a scalar potential in the Kohn-Sham Hamiltonian. This potential has a saw-tooth shape, a fact that follows from the imposition of periodic boundary conditions, and gradient of this scalar potential, which is constant across the unit-cell, is then the electric field. Due to this extra term in the Hamiltonian, the Kohn-Sham eigenvalues and eigenvectors are modified. These quantities then lead to an implicit presence of the electric-field in the single particle Green’s function G0 and the RPA dielectric function (i.e. the screening), ε−1, and hence the screened Coulomb potential W0 = ε−1v.
How to cite this article: Azhikodan, D. et al. An anomalous interlayer exciton in MoS2. Sci. Rep. 6, 37075; doi: 10.1038/srep37075 (2016).
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Butler, S. Z. et al. Progress, challenges, and opportunities in two-dimensional materials beyond graphene. ACS Nano 7, 2898–2926 (2013).
Chhowalla, M. et al. The chemistry of two-dimensional layered transition metal dichalcogenide nanosheets. Nature Chemistry 5, 263–275 (2013).
Wang, Q. H., Kalantar Zadeh, K., Kis, A., Coleman, J. N. & Strano, M. S. Electronics and optoelectronics of two-dimensional transition metal dichalcogenides. Nature Nanotechnology 7, 699–712 (2012).
Xiao, D., Liu, G.-B., Feng, W., Xu, X. & Yao, W. Coupled spin and valley physics in monolayers of MoS2 and other group-VI dichalcogenides. Phys. Rev. Lett. 108, 196802 (2012).
Chu, T., Ilatikhameneh, H., Klimeck, G., Rahman, R. & Chen, Z. Electrically tunable bandgaps in bilayer MoS2 . Nano Letters 15, 8000–8007 (2015).
Conley, H. J. et al. Bandgap engineering of strained monolayer and bilayer MoS2 . Nano Letters 13, 3626–3630 (2013).
Splendiani, A. et al. Emerging photoluminescence in monolayer MoS2 . Nano Letters 10, 1271 (2010).
Radisavljevic, B., Radenovic, A., Brivio, J., Giacometti, V. & Kis, A. Single-layer MoS2 transistors. Nature Nanotechnology 6, 147–150 (2011).
Yin, Z. et al. Single-layer MoS2 phototransistors. ACS Nano 6, 74–80 (2012).
Mak, K., Lee, C., Hone, J., Shan, J. & Heinz, T. Atomically thin MoS2: A new direct-gap semiconductor. Physical Review Letters 105, 136805–0 (2010).
Klots, A. R. et al. Probing excitonic states in suspended two-dimensional semiconductors by photocurrent spectroscopy. Scientific Reports 4, 6608– (2014).
Li, Z. et al. Active light control of the MoS2 monolayer exciton binding energy. ACS Nano 10158 (2015).
Palummo, M., Bernardi, M. & Grossman, J. C. Exciton radiative lifetimes in two-dimensional transition metal dichalcogenides. Nano Letters 15, 2794–2800 (2015).
Steinhoff, A. et al. Efficient excitonic photoluminescence in direct and indirect band gap monolayer MoS2 . Nano Letters 150831160549006– (2015).
Zhu, B., Chen, X. & Cui, X. Exciton binding energy of monolayer WS2 . Scientific Reports 5, 9218– (2015).
Hanbicki, A., Currie, G., Kioseoglou, M., Friedman, A. & Jonker, B. Measurement of high exciton binding energy in the monolayer transition-metal dichalcogenides WS2 and WSe2 . Solid State Communications 203, 16–20 (2015).
Bernardi, M., Palummo, M. & Grossman, J. C. Extraordinary sunlight absorption and one nanometer thick photovoltaics using two-dimensional monolayer materials. Nano Letters 13, 3664–3670 (2013).
Komsa, H.-P. & Krasheninnikov, A. V. Effects of confinement and environment on the electronic structure and exciton binding energy of MoS2 from first principles. Phys. Rev. B 86, 241201 (2012).
Salpeter, E. E. & Bethe, H. A. A relativistic equation for bound-state problems. Phys. Rev. B 84, 1232 (1956).
Sharma, S., Dewhurst, J. K., Sanna, A. & Gross, E. K. U. Bootstrap approximation for the exchange-correlation kernel of time-dependent density-functional theory. Phys. Rev. Lett. 107, 186401 (2011).
Molina Sanchez, A., Sangalli, D., Hummer, K., Marini, A. & Wirtz, L. Effect of spin-orbit interaction on the optical spectra of single-layer, double-layer, and bulk MoS2 . Phys. Rev. B 88, 045412 (2013).
Singh, N., Jabbour, G. & Schwingenschlögl, U. Optical and photocatalytic properties of two-dimensional MoS2 . Eur. Phys. J. B 85, 392 (2012).
Ramasubramaniam, A., Naveh, D. & Towe, E. Tunable band gaps in bilayer transition-metal dichalcogenides. Phys. Rev. B 84, 205325 (2011).
Zhang, Z. Y. et al. Indirect-direct band gap transition through electric tuning in bilayer MoS2 . The Journal of Chemical Physics 140, 174707– (2014).
Liu, Q. et al. Tuning electronic structure of bilayer MoS2 by vertical electric field: A first-principles investigation. The Journal of Physical Chemistry C 116, 21556–21562 (2012).
He, J., Hummer, K. & Franchini, C. Stacking effects on the electronic and optical properties of bilayer transition metal dichalcogenides MoS2, MoSe2, WS2, and WSe2 . Phys. Rev. B 89, 075409 (2014).
Choi, J.-H., Cui, P., Lan, H. & Zhang, Z. Linear scaling of the exciton binding energy versus the band gap of two-dimensional materials. Phys. Rev. Lett. 115, 066403 (2015).
Boker, T. et al. Band structure of MoS2, MoSe2, and α–MoTe2 angle-resolved photoelectron spectroscopy and ab initio calculations. Phys. Rev. B 64, 235305 (2001).
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 78, 1396 (1997).
Kresse, G. & Furthmuller, J. Efficient iterative schemes for ab initio total-energy calculations using a plane-wave basis set. Phys. Rev. B 54, 11169–11186 (1996).
Shishkin, M. & Kresse, G. Implementation and performance of the frequency-dependent GW method within the PAW framework. Phys. Rev. B 74, 035101 (2006).
Dewhurst, J. K., Sharma, S. et al. URL http:/elk.sourceforge.net/.
S.S acknowledges Department of Physics, Indian Institute of Technology Roorkee for the visiting position. D.A acknowledges Ministry of Human Resource Development, Government of India and the HPC facility at Max Planck Institute of Microstructure Physics, Halle, Germany.
The authors declare no competing financial interests.
Rights and permissions
This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/
About this article
Cite this article
Azhikodan, D., Nautiyal, T., Shallcross, S. et al. An anomalous interlayer exciton in MoS2. Sci Rep 6, 37075 (2016). https://doi.org/10.1038/srep37075
This article is cited by
Generating intense electric fields in 2D materials by dual ionic gating
Nature Communications (2022)
Optical control of polarization in ferroelectric heterostructures
Nature Communications (2018)
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.